ACI MATERIALS JOURNAL
Nanoindentation, quantitative modulus mapping, and PeakForce quantitative nanomechanical mapping (QNM) are applied to inves-tigate the quantitative nanomechanics of hardened cement paste at different spatial resolutions. The elastic modulus measured by static nanoindentation is slightly higher than those measured by the other methods. The average elastic modulus and probability obtained by PeakForce QNM are typically consistent with those found by modulus mapping. Both modulus mapping and Peak-Force QNM can be used to discriminate different material phases in cement paste at the nanoscale. It concludes that cement paste is a granular material in which the sub-micron scale grains or basic nanoscale units pack together. Moreover, the high resolution Peak-Force QNM can provide an efficient tool for identifying nanome-chanical properties, particle sizes, and thickness of the interface between different nanoscale grains.
Keywords: cement paste; nanoindentation; nanomechanical properties; modulus mapping; PeakForce quantitative nanomechanical mapping (QNM).
Exploring the properties of cement-based materials at the nanoscale has received much attention in recent years.1-4 Measurement of nanoscale mechanical properties of cement-based materials is necessary in understanding the phase char-acteristics, the initiation of microcracking under loading, and physical transport properties of concrete. Recently, three advanced techniques have been developed: 1) depth-sensing nanoindentation5-7; 2) quantitative modulus mapping in the form of scanning probe microscopy (SPM)8-11; and 3) atomic force microscopy (AFM)-based PeakForce quan-titative nanomechanical mapping (QNM).12-15 The capabili-ties of these instruments cover a wide range of contact areas and displacement resolutions from the sub-micron scale in nanoindentation down to nanoscale in PeakForce QNM.
Nanomechanical testing can be used to assess the mechan-ical properties of the individual constituents of heteroge-neous materials and, in this way, to provide meaningful experimental data for multi-scale numerical modeling. Nanoindentation has been a popular technique used for this purpose.16,17 In nanoindentation, the in-place imaging method allows for observing the surface topography and placing the indents at the desired locations.18,19 Statistic tech-niques have been argued to determine the elastic modulus of different phases in cement paste.20-24 During nanoindenta-tion testing, a diamond indenter is inserted into the surface of the sample, which would cause damage to the surface. As for the quantitative modulus mapping technique, the advan-tage is that the contact stiffness can be obtained continuously during scanning using a smaller contact force, which could be an ideal technique for multi-phase and composite mate-rials.10,11 PeakForce QNM has been recognized as a useful
method for the assessment of local mechanical properties of materials, which can also provide phase contrast maps for qualitative characterization of materials with a high spatial resolution.12,14
The objective of this study is to use correlative quantita-tive nanomechanical methods to measure the nanomechan-ical properties of cement paste. The relative merits of the application of these three methods are specifically discussed for the determination of elastic modulus of cement paste from one-micrometer length scale to tens of nanometers scale. This fundamental understanding will be helpful in improving the basic behaviors of concrete, such as strength and durability.
NANOMECHANICAL METHODS Nanoindentation
A static nanoindenation experiment was performed with a nanomechanical testing system equipped with an in-place imaging mode (Fig. 1). The nanoindentation instrument consists of a force-displacement transducer with electro-static force actuation and displacement sensing electronics. MS No. M-2013-237.R2
Experimental Investigation on Quantitative
Nanomechanical Properties of Cement Paste
by Wengui Li, Jianzhuang Xiao, Shiho Kawashima, Gajendra S. Shekhawat, and Surendra P. Shah
ACI Materials Journal, V. 111, No. 1-6, January-December 2014.
MS No. M-2013-237.R2 received October 28, 2013, and reviewed under Institute publication policies. Copyright © 2014, American Concrete Institute. All rights reserved, including the making of copies unless permission is obtained from the copyright proprietors. Pertinent discussion including author’s closure, if any, will be published ten months from this journal’s date if the discussion is received within four months of the paper’s print publication.
A two-dimensional Berkovich indenter with a high elastic modulus is used. The suggested Poisson’s ratio ν of the cement paste is 0.2.25 The system is calibrated with standard quartz crystal before performing the actual indentation on the sample to ensure that the probe is not contaminated or damaged.
A typical representation of the indentation load versus indentation depth or displacement for an indentation experi-ment is shown in Fig. 2. The elastic modulus E of the sample is calculated as follows S dP dh Er A = = 2 π (1) E E E s s r i i = − − − − (1 2) 1 1 2 1 ν ν (2)
where P is the indentation load; h is the indentation depth;
S is the initial unloading stiffness; A is the projected contact
area; Er is the reduced elastic modulus; Es and νs are elastic
modulus and Poisson’s ratio for the sample, respectively; and Ei and νi are the corresponding parameters for the
indenter, respectively. For the indenter used in this study, the elastic modulus Ei = 1140 GPa (165,300 ksi), and the
Pois-son’s ratio νi = 0.07. Modulus mapping
Quantitative modulus mapping in the form of SPM images is acquired using the direct force modulation (nanoDMA) operating mode of the nanomechanical testing system. The schematic representation of the instrument configuration and dynamical mode are shown in Fig. 3. A cube-corner diamond tip is attached to a force-displacement transducer. As with nanoindentation, the system was calibrated with a standard quartz crystal. A lock-in amplifier is used to analyze the sample response, yielding displacement amplitude, and the phase shift between the contact force and the displace-ment. The contact stiffness and material damping are calcu-lated from the amplitude and phase shift using a dynamic model.8,10
To apply a load, a voltage is applied to generate an elec-trostatic force Fe. The mode of the direct force modulation
applies a parallel loading configuration. The relevant equa-tion of moequa-tion is F t F t m dz dt dz dt kz e( )= sin( )= + + 0 2 2 ω β (3)
where ω is the angular frequency; F0 is the amplitude of the applied sinusoidal force; m is the mass of the moving trans-ducer; β = βi + βs is the combined damping coefficient of the
indenter and the sample; k = ki + kc is the combined stiffness
of the indenter and the sample; z is the resulting sinusoidal displacement; and t is time. The solution to this differential equation is
z = z0sin(ωt + φ) (4) where the displacement amplitude z0 is given by the dynam-ical compliance function
z F k m 0 0 2 2 2 12 =[( − ω ) +(βω) ]− (5)
where the phase φ of the displacement is dictated by
tan( )ϕ βω
ω = −
k m 2 (6)
Determination of m, β, and ki is accomplished by
nonlinear curve fitting of the dynamic compliance versus the frequency trace obtained in air. The storage K′ and loss K′′ components of the complex contact stiffness are extracted from the spatially correlated set of amplitude and phase images to generate quantitative stiffness maps
K′ = kc (7)
Fig. 2—Typical representation of indentation load versus indentation depth.19
K′′ = βcω (8)
Rearrangement of the familiar equations of Hertzian theory yields the following relationship for the contact radius a a FR K = ′ 3 2 (9)
where F corresponds to the nominal contact force, and R is the tip radius. The modulus then can be calculated as
E K a s = ′ 1 2 (10)
In static nanoindentation, a minimum separation of 3 μm (118 μin.) between indentations is required to avoid possible interactions between adjacent indentions. The modulus mapping technique in the form of scanning probe micros-copy (SPM) images, however, can overcome these short-comings. This is because the material under the tip is probed within the elastic region, and once the tip force is removed, the material can fully recover without local residual stress or permanent deformation.
Recently, a high resolution method called PeakForce QNM was developed to study the quantitative mechanical properties of cement-based materials at approximately 10 nm (0.4 μin.) resolution.14,26,27 PeakForce QNM is a mode with improved force resolution combined with real time calculation of elastic modulus at each surface contact, which can detect local elastic modulus. This technique can provide compositional mapping of a complex composite material while providing high resolution. In PeakForce tapping, the probe and sample are intermittently brought together (similar to tapping mode) to contact the surface for a short period, which eliminates lateral forces. Unlike tapping mode, where the feedback loop keeps the cantilever vibra-tion amplitude as a constant, PeakForce tapping controls the maximum force on the tip. This protects the tip and sample from damage while allowing the tip sample contact area to be minimized.
For the PeakForce QNM, the schematic diagram of the collected force-separation curve is shown in Fig. 4. To elucidate the elastic properties from the PeakForce QNM, the Derjaguin-Muller-Toporov (DMT) model can be used for the estimation of reduced elastic modulus.28 The forces during the tip-surface interaction can be described by
Fint E Rd Fadh * =4 + 3 3 (11)
where Fint is the tip-sample force during the tip-surface inter-action; E* is the combined elastic modulus of the tip and the sample; R is the tip radius; d is the sample deformation; and Fadh is the adhesion force during the contact. The elastic
modulus of the sample Es can be derived from the following
equation 1 1 2 1 2 E E E s s tip tip * = − + − ν ν (12) where νs is the Poisson’s ratio of the sample; νtip is the
Pois-son’s ratio of the tip; Es is the elastic modulus of the sample;
and Etip is the elastic modulus of the tip. Calibration was also
performed by the relative method13 using a standard quartz crystal. The testing parameters of the three techniques are listed in Table 1.
Fig. 4—PeakForce QNM schematic.3,13 Table 1—Testing parameters of three techniques
Nanoindentation Modulus mapping PeakForce QNM
Berkovich (two-dimensional, 142.3 degrees) Berkovich (one-dimensional, cube-corner) AFM cantilever
Tip radius 600 nm (23.6 μin.) — 5 nm (0.2 μin.)
Tip material Diamond Diamond Diamond
Indent depth 200 to 800 nm (8 to 32 μin.) 7 to 12 nm (0.28 to 0.47 μin.) 2 to 8 nm (0.08 to 0.32 μin.)
Radius of curvature — 557.14 nm (22 μin.) —
Applied force 1200 μN (270 × 10–6 lb) 20 μN (4.5 × 10–6 lb) 50 nN (11.2 × 10–9 lb)
Deflection sensitivity — — 70 nm/V (2.8 μin./V)
A 5 mm (0.2 in.) thick 10 x 10 mm (0.4 x 0.4 in.) block of hardened cement paste with a water-cement ratio of 0.40 was produced from Type I portland cement. The cement paste was cured for 90 days under 25°C (77°F) and 95% relative humidity condition. The sample was initially ground on paper disks with gradation of grits. One polishing method can provide repeated success by long durations of polishing under light load. An auto-polisher was used with diamond suspensions in ethanol with gradations. Each step lasted approximately 30 minutes. In the following steps, diamond lapping films with gradations were used.1,21,24 The completed polished surface is shown in Fig. 5(a). Figure 5(b) shows the surface topography of a square region of the polished sample as acquired by high-resolution tapping mode AFM. The root-mean-square (RMS) of the surface roughness based on the topography map is 93.9 ± 20 nm (3.7 ± 0.79 μin.) for a scan size of 50 x 50 μm (0.002 x 0.002 in.). The RMS value can be used to evaluate the surface roughness because there is no standard criterion of roughness of cement pastes for nanomechanical testing due to the inherent roughness of hardened cement pastes, particularly which would be appli-cable to the three methods presented.29 For nanoindenta-tion, the most commonly used method for nanomechanical characterization of cement hydration products is Miller et al.,30 who reported the RMS roughness measured over an area with one side 200 times the average depth of
indenta-tion should be less than one fifth of the average indentaindenta-tion depth. The roughness of the samples tested in this study is sufficiently low and is comparable to those obtained by other investigators.3,4,30
RESULTS AND DISCUSSION Nanoindentation
Nanoindentation was performed on the cement paste sample. During the first 5 seconds, the indenter was driven into the sample at a 240 μN/s (54 μlb/s) loading rate. After reaching the maximum load of 1200 μN/s (270 μlb/s), the indenter was held in place for 2 seconds to reduce the creep effect before unloading at a rate of 240 μN/s (54 μlb/s). Indentations were made on separate 15 x 15 μm (591 x 591 μin.) and 100 x 100 μm (0.004 x 0.004 in.) regions to compare profiles and cover more phases for statistical analysis.
Figure 6 shows typical loading and unloading curves during indentations on different phases of cement paste. The tested indentation modulus4,7 for porosity, hydrates (predom-inantly calcium silicate hydrate [C-S-H]), calcium hydroxide (CH), and unhydrated cement grains are given in Table 2. Figures 7 and 8 are contour maps of indentation modulus for the area of 100 x 100 μm (0.004 x 0.004 in.) and 15 x 15 μm (591 x 591 μin.), respectively. Results indicate the general heterogeneity of mechanical properties in the tested sample, which might be due to the different phases shown in Fig. 6. The areas with a relatively high indentation modulus value, higher than 50 GPa (7252 ksi), would be unhydrated or partially hydrated cement particles. This value is in agree-ment with the values of the elastic modulus measured exper-imentally for partially hydrated clinker residues by other researchers.3,6 The regions with indentation modulus values ranging from 10 to 50 GPa (1450 to 7252 ksi) are hydration products.6,21,31-33 The lower values of indentation modulus, less than 10 GPa (1450 ksi), are likely due to porous regions in the cement paste.20,21
Figure 9 shows the indentation modulus probability distri-bution to compare the statistical analysis of two different scanned areas. The peak modulus of the probability plot in the 15 x 15 μm (591 x 591 μin.) area is higher than that in the 100 x 100 μm (0.004 x 0.004 in.). The distribution of phases is clearly influenced by the size of the scanned area: for the larger area, the amount of cement clinker and porosity phase increase, which results in a greater variation in the
inden-Fig. 5—Cement paste sample after polishing: (a) optical image; and (b) AFM image.
Fig. 6—Load-depth diagrams of different phases in cement paste.7,20 (Note: 1 μN = 0.225 × 10–6 lb; 1 nm = 0.04 μin.)
Table 2—Typical nanomechanical properties for indented phases3,7,20
Material phase Maximum depth, nm modulus, GPaElastic Hardness, GPa Porosity 843.1 ± 127.5 4.75 ± 4.78 0.04 ± 0.21 Hydrates (primarily C-S-H) 300.9 ± 97.6 20.31 ± 12.59 0.64 ± 0.45 Calcium hydroxide (CH) 157.2 ± 50.0 55.75 ± 15.80 1.51 ± 0.67 Unhydrated cement particle 73.3 ± 37.4 89.47 ± 19.19 4.52 ± 1.57
tation modulus distribution. Although many studies have been conducted on the nanomechanical properties of phases in cement paste, little has been reported to characterize and provide quantitative measurements considering different sizes of the investigated area.
When switching the testing mode to study the nanome-chanical properties of cement paste by modulus mapping and nanoindentation in the indenter, the position of the tested sample remains unchanged. As the sample surface could potentially be damaged by the larger force required by static nanoindentation, modulus mapping was always performed first on the sample. Figure 10 shows topograph-ical maps for the areas 15 x 15 μm (591 x 591 μin.) and 5 x 5 μm (197 x 197 μin.), respectively, which were obtained by modulus mapping. It reveals that cement paste is composed of different types of phases.
Figure 11(a) shows the elastic modulus contour maps for the area of 15 x 15 μm (591 x 591 μin.). From Fig. 11(b), it is found that quantitative modulus variations in modulus mapping are larger than those in nanoindentation. The range
Fig. 7—Elastic modulus of cement paste obtained by nanoin-dentation (100 x 100 μm): (a) innanoin-dentation modulus contour map; and (b) indentation modulus distribution. (Note: 1 μm = 39.4 μin.; 1.0 GPa = 145 ksi.)
Fig. 8—Elastic modulus of cement paste obtained by nanoindentation (15 x 15 μm): (a) contour map of inden-tation modulus; and (b) indeninden-tation modulus distribution. (Note: 1 μm = 39.4 μin.; 1.0 GPa = 145 ksi.)
Fig. 9—Statistical analysis of modulus (bin size = 5.0 GPa). (Note: 1 μm = 39.4 μin.; 1.0 GPa = 145 ksi.)
of elastic moduli, from 0.2 to 124.5 GPa (29 to 18,057 ksi), is found to be significantly greater than that obtained by static nanoindentation.10,34 The results for the scanned area 5 x 5 μm (197 x 197 μin.) are shown in Fig. 12. The results reveal that the modulus mapping technique is more sensitive than static nanoindentation, as indicated by the higher spatial resolution. Significant local elastic modulus variations were observed at the sample surface, which was comprised of different phases and interfaces between hydration products. Moreover, clear abrupt changes in the elastic modulus were measured, and found to be due to the interfaces between the pores and different hydration products. The modulus proba-bility histograms for two different areas are presented in Fig. 13. It is clear that the peak modulus in the probability plot is slightly higher for the area 5 x 5 μm (197 x 197 μin.) than for 15 x 15 μm (591 x 591 μin.).
Modulus mapping and PeakForce QNM were performed on two separate devices. Thus, when switching from one method to the other, it is necessary to confirm that they are each performed at the same position on the sample. To do this, high-resolution images were captured during the test, and image analysis was performed to measure the distance and adjust the test position accordingly.
Figure 14 shows the 512 x 512 pixel topography images of two scanning areas, 5 x 5 μm and 1 x 1 μm (197 x 197 μin. and 39.4 x 39.4 μin.), of a cement paste sample obtained
Fig. 10—Surface topography obtained by modulus mapping: a) 15 x15 μm; and b) 5 x 5 μm. (Note: 1 μm = 39.4 μin.)
Fig. 11—Elastic modulus obtained by modulus mapping (15 x 15 μm): (a) modulus contour map; and (b) elastic modulus distribution. (Note: 1 μm = 39.4 μin.; 1.0 GPa = 145 ksi.)
by PeakForce QNM. The microstructural and nanostructural contrast can be observed clearly in the surface topography. It should be noted that the intrinsic porosity in cement paste poses some constraint on the use of PeakForce QNM, for which some noise could be expected. The images indicate that the height distribution of local areas varies widely for different measuring areas. The values of all local roughness, however, are actually sufficiently low for PeakForce QNM testing.3,13 The topography images also demonstrate that the cement paste is a granular material, where the sub-mi-cron scale grains or basic nanoscale units pack together densely.35-39
Clear nanostructural features for the area of 5 x 5 μm (197 x 197 μin.) that can be discerned in the contour image are presented in Fig. 15. In these images, the porosity and the interfaces between nanoscale grains appear dark with a lower elastic modulus. To analyze the nanostructure and nanomechanical properties in more detail, a smaller area of 1 x 1 μm (39.4 x 39.4 μin.) was studied, as shown in Fig. 16. Based on previous studies, the elastic modulus of the measuring area identified as the pore space is typically below 10.0 GPa (1450 ksi), while the elastic modulus of the measuring areas identified as hydration products were found to vary approximately between 10.0 and 50.0 GPa (1450 and 7252 ksi).7,40,41 The probabilities of elastic modulus for two different scanning areas are shown in Fig. 17. It demonstrates that the probability distributions do not seem to provide a very clear indication for the occurrence of different types of C-S-H. When comparing the analogous probability results of the two different scanning areas, the peak modulus value of the probability plot for the area of 5 x 5 μm (197 x 197 μin.) appears to be close to that of 1 x 1 μm (39.4 x 39.4 μin.), which is found to be approximately 25.0 ± 2.0 GPa (3626 ± 290 ksi).
As shown in Fig. 18, it is suggested that the PeakForce QNM technique can reveal the different types of grains in hardened cement paste. This observation also highlights the advantage of evaluating the interfaces between grains by detecting the elastic modulus distribution. According to the quantitative modulus value of the presented results, there is a clear jump in the elastic modulus distribution across the interfaces between grains. The elastic modulus of the grains themselves, however, typically exhibits a constant value. Moreover, abrupt changes in the elastic modulus across the interfaces were clearly observed. The information stemming
Fig. 13—Statistical analysis of modulus (bin size = 2.0 GPa). (Note: 1 μm = 39.4 μin.; 1.0 GPa = 145 ksi.)
Fig. 14—Surface topography obtained by PeakForce QNM: a) 5 x 5 μm; and b) 1 x 1 μm. (Note: 1 μm = 39.4 μin.)
Fig. 15—Elastic modulus obtained by PeakForce QNM (5 x 5 μm): (a) modulus contour map; and (b) modulus distribution. (Note: 1 μm = 39.4 μin.; 1.0 GPa = 145 ksi.)
from the PeakForce QNM technique can reasonably identify the grains with sizes from 20 to 400 nm (0.79 to 15.8 μin.) in the nanostructure. To provide quantitative measurements of the interface thickness between grains, radial lines (interface A-A, B-B, and C-C) across the grain boundaries were applied to indicate the elastic modulus variation corresponding to the interface thickness. By definition, the interface starts from the point where the elastic modulus begins to change from that of one grain, and extends to another point where the local elastic modulus is equal to that of another grain. The distance between these two points corresponds to the interface thickness. The thickness of the interface obtained by averaging these lines, and the most probable thickness of the interface between grains, was found to be 15 ± 5 nm (0.59 ± 0.2 μin.).
Based on the analyses and comparisons among the results from nanoindentation, modulus mapping, and PeakForce QNM, the following conclusions can be drawn:
1. The average modulus measured by static nanoindenta-tion is higher than those measured by the modulus mapping technique and PeakForce QNM, which may be due to the confinement effect and the plastic deformation in the nanoindentation.
2. Compared with static nanoindentation, modulus mapping allows for evaluation of local mechanical proper-ties within smaller measuring areas at the nanoscale. More-over, modulus mapping avoids influence on elastic modulus due to possible interaction between adjacent indentations.
3. The average elastic modulus and probability distribu-tion obtained from PeakForce QNM are typically consistent with those measured with quantitative modulus mapping. Compared with the modulus mapping, PeakForce QNM can provide local mechanical properties with a higher spatial resolution.
4. Different types of grains are detected with the quan-titative elastic modulus value. Obvious local interfaces between grains could be observed from the abrupt change in the mechanical properties distribution when crossing the boundary between different phase grains.
5. It is proven that cement paste is a granular material, in which the sub-micron scale grains or basic nanoscale units pack together. Moreover, the correlative nanomechanical methods provide an efficient tool for identification of prop-erties and particle sizes of grains, and the interfaces between grains.
ACI member Wengui Li is an Assistant Professor in the College of Civil Engineering at Hunan University, Changsha, Hunan, China. He received his PhD from Tongji University, Shanghai, China, in 2013, and was a Visiting Researcher at the Center for Advanced Cement-Based Materials at Northwestern University, Evanston, IL from Nov. 2010 to Jan. 2013. He is a member of ACI Committee 555, Concrete with Recycled Materials. His research interests include mechanical behaviors of cement-based materials and computer simulation.
Jianzhuang Xiao is a Professor in the Building Engineering Department at
Tongji University, and the Director of the Recycled Concrete Committee in China. His research interests include the mechanical and structural behav-iors of recycled concrete.
ACI member Shiho Kawashima is an Assistant Professor in the Depart-ment of Civil Engineering and Engineering Mechanics at Columbia University, New York, NY. Her research interests include nanomodification, nanocharacterization of cementitious materials, and sustainable infra-structural materials.
Gajendra S. Shekhawat is a Research Associate Professor, NIFTI Facility
Manager, at the International Institute for Nanotechnology, Northwestern University. His research interests include nanomaterials synthesis and characterization, surface characterization methods, and quantitative and qualitative scanning probe microscopy.
Fig. 16—Elastic modulus obtained by PeakForce QNM (1 x 1 μm): (a) modulus contour map; and (b) modulus distribution. (Note: 1 μm = 39.4 μin.; 1.0 GPa = 145 ksi.)
Fig. 17—Statistical analysis of modulus (bin size= 2.0 GPa). (Note: 1 μm = 39.4 μin.; 1.0 GPa = 145 ksi.)
Surendra P. Shah, FACI, is the Walter P. Murphy Professor of Civil
Engi-neering at Northwestern University. He is a member of ACI Committees 215, Fatigue of Concrete; 363, High-Strength Concrete; 440, Fiber-Rein-forced Polymer Reinforcement; 544, Fiber-ReinFiber-Rein-forced Concrete; 548, Poly-mers and Adhesives for Concrete; 549, Thin Reinforced Cementitious Prod-ucts and Ferrocement; S803, Faculty Network Coordinating Committee; and Joint ACI-ASCE Committee 446, Fracture Mechanics of Concrete.
The authors would like to acknowledge the financial support from the National Natural Science Foundation of China (51178340). All tests were performed in the NIFTI facility of the NUANCE Center at Northwestern University. The first author would like to thank the China Scholarship Council (CSC) and the Fund Support Project for Young Faculty at Hunan University (531107040800). The authors also gratefully thank G. Lomboy and D. J. Corr.
1. Mondal, P.; Shah, S. P.; and Marks, L. D., “Nanoscale Characteri-zation of Cementitious Materials,” ACI Materials Journal, V. 105, No. 2, Mar.-Apr. 2008, pp. 174-179.
2. Kim, J. H.; Mondal, P.; and Shah, S. P., “Cement-Based Materials Characterization at Nanoscale: Nanoindentation and Ultrasonic Atomic Force Microscopy (AFM),” Advances in the Material Science of Concrete, SP-270, American Concrete Institute, Farmington Hills, MI, 2010, pp. 67-76.
3. Trtik, P.; Kaufmann, J.; and Volz, U., “On the Use of Peak-Force Tapping Atomic Force Microscopy for Quantification of the Local Elastic Modulus in Hardened Cement Paste,” Cement and Concrete Research, V. 42, No. 1, 2012, pp. 215-221.
4. Jones, C. A.; Grasley, Z. C.; and Ohlhausen, J. A., “Measurement of Elastic Properties of Calcium Silicate Hydrate with Atomic Force Micros-copy,” Cement and Concrete Composites, V. 34, No. 4, 2012, pp. 468-477. 5. Jones, C. A., and Grasley, Z. C., “Short-Term Creep of Cement Paste during Nanoindentation,” Cement and Concrete Composites, V. 33, No. 1, 2011, pp. 12-18.
6. Davydov, D.; Jirásek, M.; and Kopecký, L., “Critical Aspects of Nano-Indentation Technique in Application to Hardened Cement Paste,”
Cement and Concrete Research, V. 41, No. 1, 2011, pp. 20-29.
7. Sorelli, L.; Constantinides, G.; Ulm, F.-J.; and Toutlemonde, F., “The Nano-Mechanical Signature of Ultra High Performance Concrete by Statis-tical Nanoindentation Techniques,” Cement and Concrete Research, V. 38, No. 12, 2008, pp. 1447-1456.
8. Syed Asif, S. A.; Wahl, K. J.; and Colton, R. J., “Nanoindentation and Contact Stiffness Measurement Using Force Modulation with a Capac-itive Load-Displacement Transducer,” The Review of Scientific Instruments, V. 70, No. 5, 1999, pp. 2408-2413.
9. Syed Asif, S. A.; Wahl, K. J.; Colton, R. J.; and Warren, O. L., “Quan-titative Imaging of Nanoscale Mechanical Properties Using Hybrid Nanoin-dentation and Force Modulation,” Journal of Applied Physics, V. 90, No. 3, 2001, pp. 1192-1200.
10. Balooch, G.; Marshall, G. W.; Marshall, S. H.; Warren, O. L.; Asif, S. A. S.; and Balooch, M., “Evaluation of a New Modulus Mapping Tech-nique to Investigate Microstructural Features of Human Teeth,” Journal of
Biomechanics, V. 37, No. 8, 2004, pp. 1223-1232.
11. Uskokovic, P. S.; Tang, C. Y.; Tsui, C. P.; Ignjatovic, N.; and Uskokovic, D. P., “Micromechanical Properties of Ahydroxyapatite/ Poly-L-Lactidebiocomposite Using Nanoindentation and Modulus Mapping,” Journal of the European Ceramic Society, V. 27, No. 2-3, 2007, pp. 1559-1564.
12. Young, T. J.; Monclus, M. A.; Burnett, T. L.; Broughton, W. R.; Ogin, S. L.; and Smith, P. A., “The Use of the PeakForceTM Quantitative
Nano-mechanical Mapping AFM-Based Method for High-Resolution Young’s Modulus Measurement of Polymers,” Measurement Science & Technology, V. 22, No. 12, 2011, doi: 10.1088/0957-0233/22/12/125703
13. Pittenger, B.; Erina, N.; and Su, C., “Quantitative Mechanical Prop-erty Mapping at the Nanoscale with PeakForce QNM,” Application Note
Veeco Instruments Inc, http://www.bruker-axs.com/uploads/AN128.pdf.
14. Vanlandingham, M. R.; McKnight, S. H.; Palmese, G. R.; Elings, J. R.; Huang, X.; Bogetti, T. A.; Eduljee, R. F.; and Gillespie Jr., J. W., “Nanoscale Indentation of Polymer Systems Using the Atomic Force Microscope,” The Journal of Adhesion, V. 64, No. 1-4, 1997, pp. 31-59.
15. Sahin, O., and Erina, N., “High-Resolution and Large Dynamic Range Nanomechanical Mapping in Tapping-Mode Atomic Force Microscopy,”
Nanotechnology, V. 19, No. 44, 2008, doi: 10.1088/0957-4484/19/44/445717
16. Xiao, J. Z.; Li, W. G.; Corr, D. J.; and Shah, S. P., “Simulation Study on the Stress Distribution in Modeled Recycled Aggregate Concrete under Uniaxial Compression,” Journal of Materials in Civil Engineering, ASCE, V. 25, No. 4, 2013, pp. 504-518.
17. Xiao, J. Z.; Li, W. G.; Corr, D. J.; and Shah, S. P., “Effects of Inter-facial Transition Zones on the Stress-Strain Behavior of Modeled Recy-cled Aggregate Concrete,” Cement and Concrete Research, V. 52, 2013, pp. 82-99.
18. Lee, J. W., and Duh, J. G., “Nanomechanical Properties Evaluation of Chromium Nitride Films by Nanoindentation and Nanowear Techniques,”
Surface and Coatings Technology, V. 188-189, 2004, pp. 655-661.
19. Oliver, W. C., and Pharr, G. M., “Improved Technique for Deter-mining Hardness and Elastic Modulus Using Load and Displacement Sensing Indentation Experiments,” Journal of Materials Research, V. 7, No. 6, 1992, pp. 1564-1583.
20. Ulm, F. J.; Vandamme, M.; Bobko, C.; and Ortega, J. A., “Statistical Indentation Techniques for Hydrated Nanocomposites: Concrete, Bone, and Shale,” Journal of the American Ceramic Society, V. 90, No. 9, 2007, pp. 2677-2692.
21. Xiao, J. Z.; Li, W. G.; Sun, Z. H.; Lange, D. A.; and Shah, S. P., “Properties of Interfacial Transition Zones in Recycled Aggregate Concrete Tested by Nanoindentation,” Cement and Concrete Composites, V. 37, 2013, pp. 276-292.
22. Mondal, P.; Shah, S. P.; and Marks, L. P., “Nanomechanical Prop-erties of Interfacial Transition Zone in Concrete,” Nanotechnology in
Construction 3: Proceedings of the NICOM3, 2009, pp. 315-320.
23. Wang, X. H.; Jacobsen, S.; He, J. Y.; Zhang, Z. L.; Lee, S. F.; and Lein, H. L., “Application of Nanoindentation Testing to Study the Inter-facial Transition Zone in Steel Fiber Reinforced Mortar,” Cement and
Concrete Research, V. 39, No. 8, 2009, pp. 701-715.
24. Li, W. G.; Xiao, J. Z.; Sun, Z. H.; Kawashima, S.; and Shah, S. P., “Interfacial Transition Zones in Recycled Aggregate Concrete with Different Mixing Approaches,” Construction & Building Materials, V. 35, 2012, pp. 1045-1055.
25. Lee, K. M., and Park, J. H., “A Numerical Model for Elastic Modulus of Concrete Considering Interfacial Transition Zone,” Cement and Concrete
Research, V. 38, No. 3, 2008, pp. 396-402.
26. Rabe, U.; Janser, K.; and Arnold, W., “Vibrations of Free and Surface-Coupled Atomic Force Microscope Cantilevers: Theory and
Fig. 18—DMT modulus obtained by PeakForce QNM (0.25 x 0.25 μm): (a) interface position; and (b) modulus distribution. (Note: 1 μm = 39.4 μin.; 1.0 GPa = 145 ksi.)
Experiment,” The Review of Scientific Instruments, V. 67, No. 9, 1996, pp. 3281-3293.
27. Sahin, O.; Magonov, S.; Su, C.; Quate, C. F.; and Solgaard, O., “An Atomic Force Microscope Tip Designed to Measure Time-Varying Nano-mechanical Forces,” Nature Nanotechnology, V. 2, 2007, pp. 507-514.
28. Derjaguin, B. V.; Muller, V. M.; and Toporov, Y. P., “Effect of Contact Deformations on the Adhesion of Particles,” Journal of Colloid and
Inter-face Science, V. 53, No. 2, 1975, pp. 314-326.
29. Trtik, P.; Dual, J.; Muench, B.; and Holzer, L., “Limitation in Obtain-able Surface Roughness of Hardened Cement Paste: Virtual Topographic Experiment Based on Focused Ion Beam Nanotomography Datasets,”
Journal of Microscopy, V. 6, No. 4, 2001, pp. 311-316.
30. Miller, M.; Bobko, C.; Vandamme, M.; and Ulm, F. J., “Surface Roughness Criteria for Cement Paste Nanoindentation,” Cement and
Concrete Research, V. 38, No. 4, 2008, pp. 467-476.
31. Jennings, H. M.; Thomas, J. J.; Gevrenov, J. S.; Constantinides, G.; and Ulm, F. J., “A Multi-Technique Investigation of the Nanoporosity of Cement Paste,” Cement and Concrete Research, V. 37, No. 3, 2007, pp. 329-336.
32. Vandamme, M.; Ulm, F. J.; and Fonollosa, P., “Nanogranular Packing of C-S-H at Substochiometric Conditions,” Cement and Concrete Research, V. 40, No. 1, 2010, pp. 14-26.
33. Alizadeh, R.; Beaudoin, J. J.; and Raki, L. R., “Mechanical Properties of Calcium Silicate Hydrates,” Materials and Structures, V. 44, No. 1, 2011, pp. 13-28.
34. Kim, J. H.; Balogun, O.; and Shah, S. P., “Atomic Force Acoustic Microscopy to Measure Nanoscale Mechanical Properties of Cement
Pastes,” Journal of the Transportation Research Board, V. 2141, 2010, pp. 102-108.
35. Masoero, E.; Del Gado, E.; Pellenq, R. J.-M.; Ulm, F. J.; and Yip, S., “Nanostructure and Nanomechanics of Cement: Polydisperse Colloidal Packing,” Physical Review Letters, V. 109, No. 15, 2012, doi: 10.1103/ PhysRevLett.109.155503
36. Brehm, D., “Size Diversity in Cement Nanoparticles Opti-mizes Packing Density to Give Concrete Its Strength,” Department of Civil and Environmental Engineering (CEE), Massachusetts Institute of Technology, Nov. 8, 2012, http://cee.mit.edu/news/releases/2012/ cement-particle-packing-density.
37. Pellenq, R. J. M.; Kushima, A.; Shahsavari, R.; Van Vliet, K. J.; Buehler, M. J.; Yip, S.; and Ulm, F. J., “A Realistic Molecular Model of Cement Hydrates,” Proceedings of the National Academy of Sciences of the
United States of America, V. 106, No. 38, 2009, pp. 16102-16107.
38. Allen, A. J.; Thomas, J. J.; and Jennings, H. M., “Composition and Density of Nanoscale Calcium-Silicate-Hydrate in Cement,” Nature
Materials, V. 6, 2007, pp. 311-316.
39. Fonseca, P. C.; Jennings, H. M.; and Andrade, J. E., “A Nanoscale Numerical Model of Calcium Silicate Hydrate,” Mechanics of Materials, V. 43, No. 8, 2011, pp. 408-419.
40. DeJong, M. J., and Ulm, F.-J., “The Nanogranular Behavior of C-S-H at Elevated Temperatures (up to 700°C),” Cement and Concrete Research, V. 37, No. 1, 2007, pp. 1-12.
41. Constantinides, G., and Ulm, F.-J., “The Nanogranular Nature of C-S-H,” Journal of the Mechanics and Physics of Solids, V. 55, No. 1, 2007, pp. 64-90.